Presentation on theme: "Metals Part 1 Manufacturing Processes, 1311 Dr Simin Nasseri Southern Polytechnic State University."— Presentation transcript:
Metals Part 1 Manufacturing Processes, 1311 Dr Simin Nasseri Southern Polytechnic State University
Manufacturing Processes Prof Simin Nasseri Four Types of Engineering Materials 1.Metals 2.Ceramics 3.Polymers 4.Composites
Manufacturing Processes Prof Simin Nasseri METALS 1.Alloys and Phase Diagrams 2.Ferrous Metals 3.Nonferrous Metals 4.Superalloys 5.Guide to the Processing of Metals
Manufacturing Processes Prof Simin Nasseri Why Metals Are Important High stiffness and strength ‑ can be alloyed for high rigidity, strength, and hardness Toughness ‑ capacity to absorb energy better than other classes of materials Good electrical conductivity ‑ Metals are conductors Good thermal conductivity ‑ conduct heat better than ceramics or polymers Cost – the price of steel is very competitive with other engineering materials
Manufacturing Processes Prof Simin Nasseri Starting Forms of Metals used in Manufacturing Processes Cast metal - starting form is a casting Wrought metal - the metal has been worked or can be worked after casting Powdered metal - starting form is very small powders for conversion into parts using powder metallurgy techniques
Manufacturing Processes Prof Simin Nasseri Classification of Metals Ferrous ‑ those based on iron Steels Cast irons Nonferrous ‑ all other metals Aluminum, magnesium, copper, nickel, titanium, zinc, lead, tin, molybdenum, tungsten, gold, silver, platinum, and others Superalloys
Manufacturing Processes Prof Simin Nasseri Metals and Alloys An Alloy = A metal composed of two or more elements At least one element is metallic Enhanced properties versus pure metals Strength Hardness Corrosion resistance Two main categories Solid Solutions Intermediate Phases
Manufacturing Processes Prof Simin Nasseri An alloy in which one element is dissolved in another to form a single ‑ phase structure Base element is metallic (Solvent) Dissolved element, metallic or non-metal Solid Solutions A phase = any homogeneous mass of material, such as a metal, in which the grains all have the same crystal lattice structure! What is a phase (in a material structure)?
Manufacturing Processes Prof Simin Nasseri Two Forms of Solid Solutions Substitutional solid solution - atoms of solvent element are replaced in its unit cell by dissolved element Interstitial solid solution - atoms of dissolving element fit into vacant spaces between base metal atoms in the lattice structure In both forms, the alloy structure is generally stronger and harder than either of the component elements Figure 6.1 Atomic radii must be similar Lower valence metal is usually solvent Must be small atoms: Hydrogen, Carbon, Nitrogen, Boron
Manufacturing Processes Prof Simin Nasseri Two Forms of Solid Solutions Substitutional solid solution Zinc dissolved in Copper = ?? Interstitial solid solution Carbon dissolved in Iron = ?? Figure 6.1 BrassSteel
Manufacturing Processes Prof Simin Nasseri Intermediate Phases There are usually limits to the solubility of one element in another When the amount of the dissolving element in the alloy exceeds the solid solubility limit of the base metal, a second phase forms in the alloy The term intermediate phase is used to describe it because its chemical composition is intermediate between the two pure elements Its crystalline structure is also different from those of the pure metals
Manufacturing Processes Prof Simin Nasseri Types of Intermediate Phases 1.Metallic compounds – consist of a metal and nonmetal, such as Fe 3 C 2.Intermetallic compounds ‑ two metals that form a compound, such as Mg 2 Pb In some alloy compositions, the intermediate phase is mixed with the primary solid solution to form a two ‑ phase structure Some two ‑ phase alloys are important because they can be heat treated for much higher strength than solid solutions
Manufacturing Processes Prof Simin Nasseri Phase Diagrams A graphical picture showing the phases of a metal alloy system as a function of composition and temperature A phase diagram for an alloy system consisting of two elements at atmospheric pressure is called a binary phase diagram Composition is plotted on the horizontal axis and temperature on the vertical axis Any point in the diagram indicates the overall composition and the phase or phases present at the given temperature under equilibrium conditions
Manufacturing Processes Prof Simin Nasseri Copper-Nickel (Cu- Ni) Phase Diagram Figure 6.2 Phase diagram for the copper ‑ nickel alloy system. solid + liquid Consider point A: Composition: 60% Ni, 40% Cu At C (or 2000 o F) the alloy is still at solid stage. Consider point B: About 35% Ni and 65% Cu, At 1250 o C, it is a mixture of liquid and solid.
Manufacturing Processes Prof Simin Nasseri Chemical Compositions of Phases The overall composition of the alloy is given by its position along the horizontal axis However, the compositions of liquid and solid phases are not the same These compositions can be found by drawing a horizontal line at the temperature of interest Where the line intersects the solidus and liquidus indicates the compositions of solid and liquid phases, respectively. We use the Inverse Lever Rule to find the compositions:
Manufacturing Processes Prof Simin Nasseri Example Determine compositions of liquid and solid phases in the Cu-Ni system at an aggregate composition of 50% nickel and a temperature of 1260 o C (2300 o F) The proportion of solid phase present is given by S phase proportion = = (50-36)/(14+12)=54% And the proportion of liquid phase present is given by L phase proportion = = 100% - 54%= 46% 100 * *
Manufacturing Processes Prof Simin Nasseri Tin-Lead Phase Diagram Figure 6.3 Phase diagram for the tin ‑ lead alloy system. Widely used in soldering for making electrical connections Molten Tin and lead Solid Tin and lead Solid Tin and molten mixture Soli lead and molten mixture Solid solution of Tin in Lead Solid solution of Lead in Tin Pure tin melts at 232 C (449 F) Pure lead melts at 327 C (621 F)
Manufacturing Processes Prof Simin Nasseri Ferrous Metals Based on iron, one of the oldest metals known to man Ferrous metals of engineering importance are alloys of iron and carbon These alloys divide into two major groups: Steel Cast iron Together, they constitute approximately 85% of the metal tonnage in the United States
Manufacturing Processes Prof Simin Nasseri Steel and Cast Iron What is the difference between steel and cast iron?!
Manufacturing Processes Prof Simin Nasseri Steel and Cast Iron Defined Steel = an iron ‑ carbon alloy containing from 0.02% to 2.1% carbon Cast iron = an iron ‑ carbon alloy containing from 2.1% to about 4% or 5% carbon Steels and cast irons can also contain other alloying elements besides carbon
Manufacturing Processes Prof Simin Nasseri Iron-Carbon Phase Diagram Figure 6.4 Phase diagram for iron ‑ carbon system, up to about 6% carbon. Watch the DVD of the book: Choose Additional Processes, then Heat treating.
Manufacturing Processes Prof Simin Nasseri Steel An alloy of iron containing from 0.02% and 2.11% carbon by weight Often includes other alloying elements: nickel, manganese, chromium, and molybdenum Steel alloys can be grouped into four categories: 1.Plain carbon steels 2.Low alloy steels 3.Stainless steels 4.Tool steels
Manufacturing Processes Prof Simin Nasseri Plain Carbon Steels Carbon is the principal alloying element, with only small amounts of other elements (about 0.5% manganese is normal) Strength of plain carbon steels increases with carbon content, but ductility is reduced High carbon steels can be heat treated to form martensite, making the steel very hard and strong Carbon StrengthCarbon Ductility
Manufacturing Processes Prof Simin Nasseri Figure 6.12 Tensile strength and hardness as a function of carbon content in plain carbon steel (hot rolled). Hardness is the characteristic of a solid material expressing its resistance to permanent deformation. It is expressed as Brinell hardness number or BHN or HB: P = applied force (kgf) D = diameter of indenter (mm) d = diameter of indentation (mm)
Manufacturing Processes Prof Simin Nasseri AISI-SAE Designation Scheme Specified by a 4 ‑ digit number system: 10XX, where 10 indicates plain carbon steel, and XX indicates carbon % in hundredths of percentage points For example, 1020 steel contains 0.20% C Developed by American Iron and Steel Institute (AISI) and Society of Automotive Engineers (SAE), so designation often expressed as AISI 1020 or SAE 1020
Manufacturing Processes Prof Simin Nasseri Plain Carbon Steels 1.Low carbon steels - contain less than 0.20% C Applications: automobile sheetmetal parts, plate steel for fabrication, railroad rails 2.Medium carbon steels - range between 0.20% and 0.50% C Applications: machinery components and engine parts such as crankshafts and connecting rods 3.High carbon steels - contain carbon in amounts greater than 0.50% Applications: springs, cutting tools and blades, wear-resistant parts
Manufacturing Processes Prof Simin Nasseri Low Alloy Steels Iron ‑ carbon alloys that contain additional alloying elements in amounts totaling less than 5% by weight Mechanical properties superior to plain carbon steels for given applications Higher strength, hardness, wear resistance, toughness, and more desirable combinations of these properties Heat treatment is often required to achieve these improved properties Large diameter pipeline
Manufacturing Processes Prof Simin Nasseri AISI-SAE Designation Scheme AISI ‑ SAE designation uses a 4 ‑ digit number system: YYXX, where YY indicates alloying elements, and XX indicates carbon % in hundredths of % points Examples: 13XX - Manganese steel 20XX - Nickel steel 31XX - Nickel ‑ chrome steel 40XX - Molybdenum steel 41XX - Chrome ‑ molybdenum steel
Manufacturing Processes Prof Simin Nasseri Stainless Steel (SS) Highly alloyed steels designed for corrosion resistance Principal alloying element is Chromium, usually greater than 15% Cr forms a thin oxide film that protects surface from corrosion Nickel (Ni) is another alloying ingredient in certain SS to increase corrosion protection Carbon is used to strengthen and harden SS, but high C content reduces corrosion protection since chromium carbide forms to reduce available free Cr Carbon StrengthCarbon Corrosion protection
Manufacturing Processes Prof Simin Nasseri Properties of Stainless Steels In addition to corrosion resistance, stainless steels are noted for their combination of strength and ductility While desirable in many applications, these properties generally make stainless steel difficult to work in manufacturing Significantly more expensive than plain C or low alloy steels
Manufacturing Processes Prof Simin Nasseri Types of Stainless Steel Classified according to the predominant phase present at ambient temperature: 1.Austenitic stainless ‑ typical composition 18% Cr and 8% Ni 2.Ferritic stainless ‑ about 15% to 20% Cr, low C, and no Ni 3.Martensitic stainless ‑ as much as 18% Cr but no Ni, higher C content than ferritic stainless
Manufacturing Processes Prof Simin Nasseri Designation Scheme for Stainless Steels Three ‑ digit AISI numbering scheme First digit indicates general type, and last two digits give specific grade within type Examples: Type 302 – Austenitic SS 18% Cr, 8% Ni, 2% Mn, 0.15% C Type 430 – Ferritic SS 17% Cr, 0% Ni, 1% Mn, 0.12% C Type 440 – Martensitic SS 17% Cr, 0% Ni, 1% Mn, 0.65% C
Manufacturing Processes Prof Simin Nasseri Additional Stainless Steels Stainless steels developed in early 1900s Several additional high alloy steels have been developed and are also classified as stainless steels: 4.Precipitation hardening stainless ‑ typical composition = 17% Cr and 7%Ni, with additional small amounts of alloying elements such as Al, Cu, Ti, and Mo (Aerospace applications) 5.Duplex stainless ‑ mixture of austenite and ferrite in roughly equal amounts (heat exchangers, pumps)
Manufacturing Processes Prof Simin Nasseri Tool Steels A class of (usually) highly alloyed steels designed for use as industrial cutting tools, dies, and molds To perform in these applications, they must possess high strength, hardness, wear resistance, and toughness under impact Tool steels are heat treated
Manufacturing Processes Prof Simin Nasseri AISI Classification of Tools Steels T, M High ‑ speed tool steels ‑ cutting tools in machining H Hot ‑ working tool steels ‑ hot ‑ working dies for forging, extrusion, and die ‑ casting D Cold ‑ work tool steels ‑ cold working dies for sheetmetal pressworking, cold extrusion, and forging W Water ‑ hardening tool steels ‑ high carbon but little else S Shock ‑ resistant tool steels ‑ tools needing high toughness, as in sheetmetal punching and bending P Mold steels ‑ molds for molding plastics and rubber
Manufacturing Processes Prof Simin Nasseri Cast Irons Iron alloys containing from 2.1% to about 4% carbon and from 1% to 3% silicon This composition makes them highly suitable as casting metals Tonnage of cast iron castings is several times that of all other cast metal parts combined, excluding cast ingots in steel-making that are subsequently rolled into bars, plates, and similar stock Overall tonnage of cast iron is second only to steel among metals
Manufacturing Processes Prof Simin Nasseri Question What do you think this is? Cross-section of a gray cast iron using an optical microscopy (up to 1000 times magnification)
Manufacturing Processes Prof Simin Nasseri Types of Cast Irons Most important is gray cast iron Other types include ductile iron, white cast iron, malleable iron, and various alloy cast irons Ductile and malleable irons possess chemistries similar to the gray and white cast irons, respectively, but result from special processing treatments Gray cast Iron Special melting and pouring treatment (Chemical treatment) Ductile Iron White cast Iron Heat treatment Malleable Iron
Manufacturing Processes Prof Simin Nasseri Cast Iron Chemistries Figure 6.13 Carbon and silicon % for cast irons, compared to steels (most steels have relatively low Si % ‑ cast steels have higher Si %). Ductile iron is formed by special melting and pouring treatment of gray cast iron. Malleable iron is formed by heat treatment of white cast iron.